AIP Advances **4, 067118 (2014); https://doi.org/10.1063/1.4882176** **4, 067118**

© 2014 Author(s).

**Correlating electroluminescence**

**characterization and physics-based models**

**of InGaN/GaN LEDs: Pitfalls and open issues**

Cite as: AIP Advances **4, 067118 (2014); **https://doi.org/10.1063/1.4882176

Submitted: 05 December 2013 . Accepted: 28 May 2014 . Published Online: 05 June 2014

Marco Calciati, Michele Goano, Francesco Bertazzi, Marco Vallone, Xiangyu Zhou, Giovanni Ghione, Matteo Meneghini, Gaudenzio Meneghesso, Enrico Zanoni, Enrico Bellotti, Giovanni Verzellesi, Dandan Zhu, and Colin Humphreys

**ARTICLES YOU MAY BE INTERESTED IN**

Efficiency droop in InGaN/GaN blue light-emitting diodes: Physical mechanisms and remedies

Journal of Applied Physics 114, 071101 (2013); https://doi.org/10.1063/1.4816434 Auger recombination in InGaN measured by photoluminescence

Applied Physics Letters 91, 141101 (2007); https://doi.org/10.1063/1.2785135 Origin of efficiency droop in GaN-based light-emitting diodes

**Correlating electroluminescence characterization**

**and physics-based models of InGaN/GaN LEDs: Pitfalls**

**and open issues**

Marco Calciati,1_{Michele Goano,}1,2,a_{Francesco Bertazzi,}1,2

Marco Vallone,1_{Xiangyu Zhou,}1_{Giovanni Ghione,}1_{Matteo Meneghini,}3

Gaudenzio Meneghesso,3_{Enrico Zanoni,}3_{Enrico Bellotti,}4

Giovanni Verzellesi,5_{Dandan Zhu,}6_{and Colin Humphreys}6
1_{Dipartimento di Elettronica e Telecomunicazioni, Politecnico di Torino,}*corso Duca degli Abruzzi 24, 10129 Torino, Italy*

2_{IEIIT-CNR, Politecnico di Torino, corso Duca degli Abruzzi 24, 10129 Torino,}*Italy*

3_{Dipartimento di Ingegneria dell’Informazione, Universit`a di Padova, Via Gradenigo 6/B,}*35131 Padova, Italy*

4_{Department of Electrical and Computer Engineering, Boston University, 8 Saint Mary’s}*Street, 02215 Boston, MA, USA*

5_{Dipartimento di Scienze e Metodi dell’Ingegneria, Universit`a di Modena e Reggio Emilia,}*42122 Reggio Emilia, Italy*

6_{Department of Materials Science and Metallurgy, University of Cambridge,}*27 Charles Babbage Road, Cambridge CB3 0FS, United Kingdom*

(Received 5 December 2013; accepted 28 May 2014; published online 5 June 2014)

Electroluminescence (EL) characterization of InGaN/GaN light-emitting diodes
(LEDs), coupled with numerical device models of different sophistication, is
rou-tinely adopted not only to establish correlations between device efficiency and
struc-tural features, but also to make inferences about the loss mechanisms responsible
for LED efficiency droop at high driving currents. The limits of this investigative
approach are discussed here in a case study based on a comprehensive set of
current-and temperature-dependent EL data from blue LEDs with low current-and high densities
of threading dislocations (TDs). First, the effects limiting the applicability of
sim-pler (closed-form and/or one-dimensional) classes of models are addressed, like
lateral current crowding, vertical carrier distribution nonuniformity, and interband
transition broadening. Then, the major sources of uncertainty affecting
state-of-the-art numerical device simulation are reviewed and discussed, including (i) the
approximations in the transport description through the multi-quantum-well active
region, (ii) the alternative valence band parametrizations proposed to calculate the
spontaneous emission rate, (iii) the difficulties in defining the Auger coefficients
due to inadequacies in the microscopic quantum well description and the
possi-ble presence of extra, non-Auger high-current-density recombination mechanisms
and/or Auger-induced leakage. In the case of the present LED structures, the
ap-plication of three-dimensional numerical-simulation-based analysis to the EL data
leads to an explanation of efficiency droop in terms of TD-related and Auger-like
*nonradiative losses, with a C coefficient in the 10*−30 cm6/s range at room
tem-perature, close to the larger theoretical calculations reported so far. However, a
study of the combined effects of structural and model uncertainties suggests that
*the C values thus determined could be overestimated by about an order of *
mag-nitude. This preliminary attempt at uncertainty quantification confirms, beyond the
present case, the need for an improved description of carrier transport and
micro-scopic radiative and nonradiative recombination mechanisms in device-level LED

a_{Electronic mail:}_{michele.goano@polito.it}

numerical models. C *2014 Author(s). All article content, except where otherwise*

*noted, is licensed under a Creative Commons Attribution 3.0 Unported License.*

[http://dx.doi.org/10.1063/1.4882176]

**I. INTRODUCTION**

The ongoing debate on efficiency droop in GaN-based light-emitting diodes (LEDs)1–6_{attests}

the present limitations of both characterization techniques and numerical models of III-nitride active
optoelectronic devices. The inadequacies of the standard drift-diffusion (DD) simulation framework
when used to describe carrier transport across a LED active region7,8 _{have elicited the inclusion}

of semiempirical corrections for mechanisms such as tunneling,9,10 carrier overflow,11,12 ballistic overshoot,13–15“nonlocal” transport between quantum wells (QWs),16and Auger-induced leakage.17 Unfortunately, the effects of those mechanisms are often hard to discriminate experimentally, which results in a problematic validation of the corresponding models. These intrinsic difficulties are compounded by at least three factors:

a. the enduring lack of reliable first-principles models for nonradiative and radiative recombination
mechanisms and other critical physical parameters (band offsets at heterojunctions,18,19_{interface}

polarization charges,20,21_{etc.) in realistic InGaN QWs,}

b. the inconsistencies in the definitions of some optical and transport parameters when used in
experimental and in simulation contexts (e.g., “bulk” Auger coefficients vs. Auger rates in
two-dimensional systems22_{),}

c. the large (but often unacknowledged) sensitivity of several key parameters to technologi-cal/structural details (interface quality, layer homogeneity, doping and composition profiles, etc.) often unaccessible to an accurate experimental determination,

to which one could add the bias towards simpler, single-mechanism explanations against more comprehensive descriptions.23–25

We set out to illustrate the main issues faced when performing a combined experimental and
simulation-based analysis of InGaN/GaN blue LEDs with an example carried out on a set of devices
grown, characterized and simulated by the authors. SectionIIdescribes the test devices and presents
the results of a systematic electroluminescence (EL) characterization for different temperatures,
essential in the determination of the relative importance of competing loss mechanisms.26_{After }

sev-eral critical structure-related issues are addressed in SectionIII(contact geometry, interplay between current crowding, current leakage and vertical nonuniformity of carrier densities, etc.), SectionIV

applies two- and three-dimensional (2D, 3D) numerical device simulation to the determination of
*“optimal” recombination parameters allowing to reproduce the experimental L/I ratio as a function*
of current density and temperature. The results of this study, leading to an explanation of efficiency
*droop in terms of Auger-like nonradiative losses characterized by a C coefficient in the 10*−30cm6_{/s}

range at room temperature, are critically discussed in SectionV, where the uncertainties and
*limita-tions of the modeling framework are shown to correspond to a possible C overestimation by about*
an order of magnitude and, more generally, underscore the problematic identification between the
*Auger-like C coefficient considered by DD analysis and the actual Auger rates. As a conclusion,*
Section VImakes briefly the case for an improved microscopic model based on a more realistic
description of the dynamics and distribution functions of carriers.

**II. STRUCTURE AND EXPERIMENTS**

In order to help discriminate the recombination coefficients, our study was carried out on two
sets of nominally identical LED structures grown on GaN templates differing for their threading
*dislocation densities (TDDs) N*disl*. Low TDD (LDD) samples have N*disl≈ 3 × 108 cm−2, while

*high TDD (HDD) devices have N*disl≈ 8 × 109 cm−2. On top of the substrate, having a 100*μm*

FIG. 1. Schematic cross-section of the LEDs under study. Only one half of the structure is reported, thanks to the symmetry
*along the lateral direction (x). The symmetry axis at the center of the mesa is represented as a dashed line. The figure is not*
*drawn to scale, since the aspect ratio W/H of the mesa is larger than 10*3_{.}

The active region, designed for 470 nm emission wavelength and non-intentionally-doped, has a
total thickness of 64 nm and includes five InGaN QWs separated by GaN quantum barriers (QBs),
with no electron or hole blocking layer (EBL/HBL). The absence of an EBL seems to have little
im-pact on the onset of droop in the devices under study; a discussion is presented in Section III.
*The epitaxial stack is completed by a 130 nm-thick GaN cap layer with p-type doping level*
3· 1019 _{cm}−3_{. From high resolution x-ray diffraction (HRXRD) spectra, the combined thickness}

of a QW/QB pair has been determined as 11.5 nm in both the LDD and HDD structures, while the In molar fraction in the QWs is in the range 0.15–0.20. As a limiting case, all simulations presented in SectionsIIIandIVwill assume in the active region an ideally piecewise constant composition profile with undoped 5 nm-thick In0.15Ga0.85N QWs and 6.5 nm-thick GaN QBs; the effects of deviations

from these values will be briefly discussed in SectionV C.

*Through an etching process, the LEDs are patterned into square mesas, having width W* =
0*.5 mm and total nominal height H = 320 nm (about 130 nm of the n-type buffer have been*

*FIG. 2. Mesh used in the 3D simulations of the LEDs under study. Thanks to the structural symmetries in the (x, y) plane,*
only one fourth of the entire device has been discretized, so that the topmost corner in the figure corresponds to the mesa
center. The anode contact (covering the top surface of the mesa) and the cathode contact (a square ring deposited on the
etched GaN buffer) are shown in purple. In order to better identify the active region, the vertical axis in the plot has been
expanded by a factor 300.

*etched). The p-type top layer is completely covered with a uniform, non-roughened semitransparent*
*square contact of area S* *= W*2*= 0.25 mm*2. Finally, a 60*μm-wide cathode contact metallization*
*is deposited on the partially exposed n-type GaN buffer, surrounding the entire mesa periphery at a*
20*μm distance from the mesa sidewalls. A schematic cross-section of the LEDs under study and a*
detail of the mesh used in the 3D simulations are shown in Figs.1and2.

*The I (V ) and L(I) characteristics (where V is the applied voltage, I is the current flowing*
*through the anode and cathode contacts, L= η*extr*P*op *is the emitted optical power, P*op is the total

optical power generated in the active region,*η*extr is the extraction efficiency) and the EL spectra

were measured under pulsed excitation over a controlled temperature range between 15 ◦C and
120 ◦C. In Fig.3 are shown the experimental EL spectra for different temperatures in the LDD
and HDD LEDs, respectively. Experimental results indicate that, predictably, LDD LEDs exhibit a
*significantly higher efficiency: the peak L/I ratio at room temperature in LDD LEDs is about twice*
as large as in HDD ones, see Fig.4. LDD devices are also affected by a much smaller temperature
*sensitivity of the quantum efficiency; for an injection current I*= 100 mA, corresponding to a current
*density J*= 40 A/cm2, a temperature increase*T = 105*◦C leads to a reduction in the emitted optical
power equal to 50% and just 10% in HDD and LDD LEDs, respectively (see Fig.5). LDD LEDs
show also a significant improvement in the stability of the peak emission wavelength *λ*peak with

respect to both temperature and injection current (see Fig.6).

**III. PRELIMINARY MODELING CONSIDERATIONS**

Our simulation analysis has been based on the APSYS modeling software from Crosslight Software Inc. and, to a lesser extent, on the TCAD SENTAURUS suite from Synopsys Inc. AP-SYS and TCAD SENTAURUS ARE WELL REPRESENTATIVE OF THE STATE OF THE ART IN OPTO -ELECTRONIC COMPUTER-AIDED DESIGN(CAD)TOOLS,WHOSE LIMITATIONS ARE THE FOCUS OF OUR INVESTIGATION. BOTHimplement 2D and 3D DD models coupled with relevant quantum corrections, including the self-consistent solution of Poisson and Schr¨odinger equations in the active region. The

4300 440 450 460 470 480 490 500 510 520
2
4
6
8
10
12
14x 10
5
Wavelength, nm
E
L
in
te
ns
it
y,
a
.u.
15*◦*_{C}
30*◦*_{C}
45*◦*C
60*◦*C
75*◦*C
90*◦*C
105*◦*_{C}
120*◦*_{C}
430 440 450 460 470 480 490 500 510 520
0
1
2
3
4
5
6
7
8
9
10x 10
6
Wavelength, nm
E
L
in
te
ns
it
y,
a
.u.
15*◦*_{C}
30*◦*_{C}
45*◦*C
60*◦*C
75*◦*C
90*◦*C
105*◦*_{C}
120*◦*_{C}
4300 440 450 460 470 480 490 500 510 520
1
2
3
4
5
6x 10
5
Wavelength, nm
E
L
in
te
ns
it
y,
a
.u.
15*◦*_{C}
30*◦*C
45*◦*C
60*◦*C
75*◦*_{C}
90*◦*_{C}
105*◦*_{C}
120*◦*C
4300 440 450 460 470 480 490 500 510 520
1
2
3
4
5
6
7x 10
6
Wavelength, nm
E
L
in
te
ns
it
y,
a
.u.
15*◦*C
30*◦*C
45*◦*C
60*◦*C
75*◦*C
90*◦*C
105*◦*C
120*◦*C

*FIG. 3. Experimental EL spectra for different temperatures in a LDD (top) and HDD (bottom) LED. I= 10 mA, J = 4 A/cm*2

*(left), I= 100 mA, J = 40 A/cm*2_{(right).}

0 5 10 15 20 25 30 35 40 0 2 4 6 8 10 12 14 16x 10 7

Current density, A/cm2

Optic
a
l
p
ow
er
,
a
.u
.
HDD 15*◦*C
HDD 45*◦*C
HDD 90*◦*C
HDD 120*◦*C
LDD 15*◦*C
LDD 45*◦*C
LDD 90*◦*C
LDD 120*◦*C
0 10 20 30 40
0
0.5
1
1.5
2
2.5x 10
9

Current density, A/cm2

E
x
te
rnal
Quan
tu
m
E
ﬃ
cie
n
cy
,
a.u
.
HDD 15*◦*C
HDD 45*◦*C
HDD 90*◦*C
HDD 120*◦*C
LDD 15*◦*C
LDD 45*◦*C
LDD 90*◦*C
LDD 120*◦*C

*FIG. 4. Measured emitted optical power (left) and corresponding experimental ratio L/I (right) as functions of the injection*
current density at different temperatures in a LDD (dashed lines) and HDD (solid lines) LED.

* valence band is described with a k· p Hamiltonian, allowing the determination of spontaneous *
emis-sion as a function of wavelength and carrier density in strained QWs; many-body effects are also
accounted for. Specific features of non-cubic semiconductors are taken into account, such as the
spontaneous and piezoelectric polarization effects, and the description of carrier transport across
the active region may be corrected with semiempirical models for e.g. tunneling and capture/escape

20 40 60 80 100 120
0.5
0.55
0.6
0.65
0.7
0.75
0.8
0.85
0.9
0.95
1
Temperature,*◦*C
Op
ti
ca
l
p
o
w
er
(n
o
rm
a
li
zed
to
1
5
*◦*C)
0.8 A/cm2
4 A/cm2
20 A/cm2
40 A/cm2
20 40 60 80 100 120
0
0.1
0.2
0.3
0.4
0.5
0.6
0.7
0.8
0.9
1
Temperature,*◦*C
Op
ti
ca
l
p
o
w
er
(n
o
rm
a
li
zed
to
1
5
*◦*C)
0.8 A/cm2
4 A/cm2
20 A/cm2
40 A/cm2

FIG. 5. Measured emitted optical power as a function of temperature at different injection current densities in a LDD (left)
*and HDD (right) LED. Each curve has been normalized with respect to its value at T*= 15◦C.

### 20

### 40

### 60

### 80

### 100

### 120

### 466

### 468

### 470

### 472

### 474

### 476

### 478

### Temperature,

*◦*

### C

### P

### ea

### k

### em

### ission

### w

### av

### ele

### n

### g

### th

### ,

### n

### m

FIG. 6. Measured*λ*peakas a function of temperature in a LDD LED (black symbols, independent of the injection current

*density) and a HDD LED (blue: J*= 4 A/cm2_{; red: 20 A/cm}2_{; green: 40 A/cm}2_{).}

processes between QWs and barriers. The nominal values of the material parameters used in the present simulations are reported in AppendixA 1.

Before addressing, in Section IV, the use of 3D simulation to extract “optimal”
*recombina-tion coefficients allowing to reproduce the experimental L/I ratios as funcrecombina-tions of current density,*
temperature and TDD, some preliminary considerations on our test devices are in order, relevant
also to most LEDs discussed in the literature.

### 0

### 50

### 100

### 150

### 200

### 250

### 0

### 10

### 20

### 30

### 40

### 50

### 60

### 70

*J*

*y*

*(x,*

*y),*

### A

### /

### cm

2*x, μm*

### LDD, 15

*◦*

### C

### LDD, 120

*◦*

### C

### HDD, 15

*◦*

### C

### HDD, 120

*◦*

### C

*FIG. 7. Simulated vertical component of the total current density Jyas a function of the lateral coordinate x (measured from*
the center of the 0.5 mm-wide mesa), across a horizontal section located 100 nm below the bottom barrier of the active region,
*at an injection current I= 100 mA (J = 40 A/cm*2_{). The current profiles J}

*y(x) in a LDD (solid lines) and HDD (dashed lines)*
*LED at T*= 15◦*C (black lines) and T*= 120◦C (red lines) are compared.

**A. Realistic spatial distribution of carriers in the active region**

*The standard ABC model used for correlating current and carrier density in the analysis of*
experimental data is:27

*I* *= qV*QW*( An+ Bn*2*+ Cn*3)*+ I*leak (1)

*where A, B, C are the “effective” Shockley-Read-Hall (SRH), radiative, and Auger recombination*
*coefficients in the QWs, q is the electron charge, V*QW *is the volume of all QWs, and I*leakaccounts

for all other loss mechanisms. This model is based on two main implicit assumptions about electron
*and hole densities n(x, y), p(x, y) in the QWs comprised into the active region: both n and p are*
*essentially constant along x and y, and n≈ p. These conditions should be satisfied also when more*
*detailed models for the ABC coefficients are used, e.g. when their possible saturation at high carrier*
densities is taken into account27,28(as a general rule, the Auger recombination rate is proportional
*to n*3only if the Maxwell-Boltzmann carrier statistics can be used, but this is not usually the case in
LEDs and lasers) or density-activated defect recombination (DADR) is considered.29Moreover, all
leakage mechanisms, including carrier overflow (thermionic emission),11,12_{non-capture by the QWs}

or ballistic overshoot,13–15_{tunneling,}9,10_{and Auger-induced leakage}17_{are usually either neglected or}

*empirically approximated with n-dependent models. Some groups have also proposed ABCD models*
to describe leakage, and numerical estimates of a third (or higher) order coefficient corresponding
to its effects have been presented e.g. in Refs.30–33.

Contrary to the one-dimensional (1D) charge-control models based on Eq. (1), a 3D DD simulation framework can take into account selfconsistently carrier nonuniformity and leakage. Therefore, it may be of general interest to discuss in detail the impact of the structural features of the

### 0

### 100

### 200

### 4.8

_{4.85}

### 4.9

_{4.95}

### 5

### 0

### 1000

### 2000

### 3000

### 4000

### 5000

### 6000

### x,

*μm*

### y,

*μm*

### Cu

### rrent

### d

### en

### si

### ty

### m

### a

### g

### ,

### A

### /

### cm

2*FIG. 8. Simulated modulus of the total current density in a LDD LED at T*= 15◦*C and I= 100 mA (J = 40 A/cm*2_{) as}

*a function of the lateral coordinate x (measured from the center of the 0.5 mm-wide mesa) and of the vertical coordinate y*
*(from the bottom of the mesa to the p side contact).*

devices under examination on the calibration of the comparison between measured and simulated characteristics.34

First, our LEDs, as well as most non-vertical structures, are affected by nonnegligible current
crowding (see e.g. Refs. 35–41). The simulated lateral profile of the vertical component of the
*electron current density Jn, y(x) in the present devices at a current I= 100 mA (J = 40 A/cm*2) is

reported in Fig.7, where a slightly stronger crowding may be observed for increasing temperature
both in the LDD and HDD case. A map of the modulus of the total current density in the mesa at the
same bias level is presented in Fig.8*, where the aspect ratio of the mesa W/H > 10*3_{is mirrored by}

*the extensions of the considered x and y intervals. Not only the current in the vicinity of the mesa*
*walls is significantly higher than the laterally averaged current reported in the L(J) and efficiency*
plots, but also carrier density levels in photogenerating regions may be significantly higher near
the sidewalls than in the case of uniform lateral distribution at the same current levels, as shown in
Fig.9. Hence, Auger-like effects could be strongly enhanced37,42–44 *and the corresponding C *
*co-efficient could be overestimated from an analysis of experimental L/I data neglecting crowding*
effects.

Second, the active region of the devices under study is not bounded by an EBL, which is
usually included in order to minimize electron leakage from the active region at high current levels.
However, in the present structure, the onset of efficiency droop may be observed at current densities
where leakage is probably still negligible. Fig.10shows that, with the selected values of material
parameters, numerical simulations predict essentially no electron leakage from the active region into
*the p-cap at a current I*= 100 mA where droop is already significant in low-TDD structures, over

### 0

### 50

### 100

### 150

### 200

### 250

### 1

### 2

### 3

### x 10

18### Ca

### rri

### er

### co

### n

### centra

### ti

### o

### n

### ,

### cm

*−*3

### 0

### 50

### 100

### 150

### 200

### 250

### 0

### 0.02

### 0.04

### R

### a

### diat

### iv

### e

### re

### com

### b

### inat

### ion,

### 1

### 0

28### cm

*−*3

### /s

FIG. 9. Simulated electron (blue solid line) and hole (red dashed-dotted line) density and corresponding radiative
*recom-bination profile (green dashed line) as a function of the lateral coordinate x (measured from the center of the 0.5 mm-wide*
*mesa), across the topmost QW of the active region of a LDD LED, at T*= 15◦*C and I= 100 mA (J = 40 A/cm*2_{).}

the entire temperature range 15–120◦C. (As discussed in Ref.45*, electron leakage may become less*
relevant for increasing temperature.) From the same figure, the importance of current crowding may
*be appreciated by comparing the Jn, y(y) profiles at different lateral coordinates.*

Third, in addition to suppressing leakage, an EBL could help achieving a more uniform
distribu-tion of carriers and EL intensity among QWs, and hence a higher efficiency. An uneven vertical carrier
distribution among QWs may have an effect similar to current crowding in enhancing Auger-like
recombination mechanisms. In fact, lateral and vertical carrier nonuniformities translate collectively
in a “reduced effective volume” of the active region, as discussed e.g. in Ref.46. In order to check
the possible effects of an EBL in the LEDs considered in the present study, a set of simulations has
been performed on a structure including a 50 nm-thick Al0.2Ga0.8N layer with a 1018cm−3*p doping*

density. (See e.g. Refs.24and47for discussions on the optimal choice of EBL thickness,
composi-tion and doping level.) Little impact from the EBL insercomposi-tion has been observed in the simulacomposi-tions,
*up to a current I*= 100 mA (see Fig.11), either on leakage current and vertical carrier distribution
or on current crowding.

As a final note in this discussion of carrier density distributions, we recall that realistic device
modeling requires the inclusion of temperature-dependent incomplete dopant ionization. In the
*present study, activation energies ED= 20 meV and EA* = 200 meV have been assumed in GaN

for Si and Mg, respectively. These energies correspond to ionized donor and acceptor densities in
*the n-buffer and p-cap N _{D}*+

*≈ 1.7 · 10*18

*18*

_{, 2 · 10}_{cm}−3

*−*

_{and N}*A* *≈ 2.7 · 10*17*, 10*18cm−3*at T*= 15◦C

*and T*= 120◦C, respectively. An example of the importance of incomplete ionization is presented in
Fig.12*, where the significant increase of the fraction of ionized acceptors at T*= 120◦C contributes
to more uniform distributions of carriers and radiative emission among the QWs of a LDD LED,48

which partly compensate the adverse effects of temperature on IQE through increased nonradiative recombination coefficients and decreased radiative processes.

### 0

### 0.05

### 0.1

### 0.15

### 0

### 10

### 20

### 30

### 40

### 50

### 60

### 70

*J*

*n,*

*y*

*(x,*

*y),*

### A

### /

### cm

2*y, μm*

*x = 249 μm, 15*

*◦*

_{C}

*x = 150 μm, 15*

*◦*

_{C}

*x = 249 μm, 120*

*◦*

_{C}

*x = 150 μm, 120*

*◦*

_{C}

*FIG. 10. Simulated vertical component of the electron current density across the active region of a LDD LED at T*= 15◦C
*(black lines) and T*= 120◦*C (red lines), at an injection current I= 100 mA (J = 40 A/cm*2_{). The current profiles at two}

*values of the lateral coordinate x (measured from the center of the 0.5 mm-wide mesa) are reported.*

**B. Structural symmetries and the 2D approximation**

A seemingly trivial simulation detail is the appropriate assignement of the boundary conditions
on the mesa walls. In the present 2D simulations, in order to halve the computational box, the
*device symmetry along the lateral direction (x) has been exploited by applying Neumann boundary*
*conditions along a vertical axis at the center of the mesa, where the reference x* = 0 has been
taken (see Figs.1and2). While the effect of this halving on the current flow across the device is
obvious, the impact on the corresponding emitted optical power must be checked in order to avoid
possible double counting, depending on the definition used by the CAD software for the power
generated/emitted from spontaneous emission.49

A less trivial symmetry issue is related to the square-ring shape of the cathode contact.
*Since the n-side metallization surrounds the entire mesa periphery, in the presence of current*
crowding a fully 3D simulation should be required.7,38,50–55 Thanks to the device symmetries
and lateral dimensions, in the following Sections a quasi-3D approximation has been adopted
*by determining temperature-dependent correction factors fJ,ring(T ; V )= J3D(T ; V )/J2D(T ; V ) and*

*fL,ring(T ; V )= L3D(T ; V )/L2D(T ; V ), used to weight the 2D-simulated current density and *

emit-ted optical power when compared with the corresponding experimental values. This
approxima-tion has been validated against fully-3D simulaapproxima-tions performed with TCAD SENTAURUS on
in-creasingly realistic test structures (see Figs. 2 and 13). The severe current crowding predicted
by both APSYS and TCAD SENTAURUS for the LED structures under consideration lead to
*fJ,ring(T ; V )≈ fL,ring(T ; V )*≈ 2 (see Fig. 14). The use of uncorrected 2D models to fit

experi-mental results in LEDs affected by current crowding may result in significant underestimation of the Auger-like recombination coefficients, as examined in the next Section. It is worth emphasizing that, however important, this modeling error can be easily prevented, and should not be confused

### 0

### 0.05

### 0.1

### 0.15

### 0

### 10

### 20

### 30

### 40

### 50

### 60

*J*

*n,*

*y*

*(x,*

*y),*

### A

### /

### cm

2*y, μm*

*x = 249 μm, no EBL*

*x = 150 μm, no EBL*

*x = 249 μm, with EBL*

*x = 150 μm, with EBL*

*FIG. 11. Simulated vertical component of the electron current density across the active region of a LDD LED at T*= 15◦C
*without (solid lines) and with (dashed lines) a 50 nm-thick p-doped Al*0.2Ga0.8*N EBL, at an injection current I= 100 mA (J*

= 40 A/cm2_{). The current profiles at two values of the lateral coordinate x (measured from the center of the 0.5 mm-wide}

mesa) are reported.

*with the possible sources of C overestimation mentioned in Section*III A(mainly concerning 1D
approximations) and the most critical ones discussed in SectionsV BandV C.

**IV. 3D SIMULATION STUDY**

Either with a charge-control model based on Eq.(1)or with a 3D numerical device simulator,
*it is straightforward to match a single experimental L/I curve of any given LED by adjusting the*
*recombination parameters ABC. Unfortunately, such an exercise is of modest practical relevance,*
because of non insignificant concerns about the uniqueness of the “optimal” coefficients determined
by the fitting process.

In the present study, the availability of experimental information not only on a wide range of
injection currents and temperatures, but also on samples differing nominally only for their TDD
(and hence for their SRH lifetimes) has allowed the definition of a large set of constraints, hopefully
removing much of the arbitrariness from the optimization procedure leading to the appraisal of the
*recombination coefficients. As additional self-imposed restrictions, the coefficients Cn, Cp*, used in

*the simulations to describe the Auger-like recombination rate as R*Auger*= n*2*pCn+ np*2*Cp*, were

*assumed to exhibit the approximately linear dependence on T observed in Refs.*67and68, while the
*A coefficient was assumed to be roughly proportional to N*disl69 (see also the recent studies on the

impact of TDD on LED efficiency presented in Refs.63,70–76). Auger coefficients were not forced
to be the same in LDD and HDD LEDs because, although nominally identical, secondary ion mass
spectrometry (SIMS) measures suggest that the QWs of the LDD devices have probably a smoother
profile, which could imply a lower Auger rate.77_{The radiative recombination coefficient B was not}

0.020 0.04 0.06 0.08 0.1 0.12 0.14
1
2
3
4
5
6
7
8
*n*
,1
0
18
cm
*−*
3
*y, μm*
LDD, 15*◦*C
LDD, 120*◦*_{C}
0.020 0.04 0.06 0.08 0.1 0.12 0.14
2
4
6
8
10
12
*p,1*
0
18
cm
*−*
3
*y, μm*
LDD, 15*◦*C
LDD, 120*◦*C
0.020 0.04 0.06 0.08 0.1 0.12 0.14
0.01
0.02
0.03
0.04
0.05
0.06
*R*ra
d
,1
0
28
cm
*−*
3*/s*
*y, μm*
LDD, 15*◦*C
LDD, 120*◦*C
0.04 0.05 0.06 0.07 0.08 0.09 0.1 0.11 0.12
0.5
1
1.5
2
2.5
3
3.5
4
4.5
5
En
er
g
y,
eV
*y, μm*

FIG. 12. Simulated electron and hole density and corresponding radiative recombination profile across the active region
*in x= 240 μm at T = 15*◦*C (black solid lines) and T*= 120◦*C (red dashed lines) for a current density J*= 40 A/cm2

*(corresponding to I*= 100 mA) in a LDD LED. (Similar profiles have been observed in the simulation of a HDD LED.) A
*detail of the band diagram at T*= 15◦*C, J*= 40 A/cm2_{is also presented, including the two lowest-lying subbands in each}

QW, the modulus of the corresponding wavefunctions, and the electron and hole quasi-Fermi levels (red dashed lines).

FIG. 13. Alternative 3D structures simulated in order to validate the standard 2D analysis and to estimate the correction
*factors fJ,ringand fL,ring. (Left) the cathode contact is placed only along the mesa walls parallel to the y axis. (Right) the*
*entire structure is assumed to be uniform along y, in complete analogy with 2D simulations.*

determined by the simulator in the active region. The optimization space was effectively limited
also by the absence of an EBL and by the seeming negligible contribution of leakage in the devices
under study, discussed in SectionIII, which remove possible effects from e.g. uncertainties in the
valence band offset at the barrier/EBL interface.45_{Some effects of model and structural parameter}

variability will be addressed in SectionV.

The “optimal” SRH lifetimes and Auger-like coefficients, determined with the nominal values of all other material parameters listed in AppendixA 1, are reported in TableIalong with previous estimates of the recombination coefficients for InGaN/GaN LEDs (see also Refs.78and79). Both

### 3

### 3.5

### 4

### 4.5

### 5

### 1.6

### 1.7

### 1.8

### 1.9

### 2

### 2.1

### 2.2

### 2.3

*V*

bias### , V

*f*

*J,ring*

### =

*J*

3D*/J*

2D
*f*

*L,ring*

### =

*L*

3D*/L*

2D
*FIG. 14. Correction factors fJ,ringand fL,ringat T*= 15◦C as functions of the applied bias.

TABLE I. Threading dislocation density, Shockley-Read-Hall lifetime*τSRH*and recombination coefficients estimated in the
present study and reported in the literature for InGaN/GaN LEDs.

*N*disl, cm−2 *τ*SRH, ns *B, cm*3/s *C, cm*6/s *λ*peak, nm
LDD, 15◦C 3· 108 _{900} _{2.7}_{· 10}−30 _{470}
LDD, 120◦C 3· 108 90 3.5· 10−30 470
HDD, 15◦C 8· 109 _{15} _{5.7}_{· 10}−30 _{470}
HDD, 120◦C 8· 109 2.7 7.8· 10−30 470
Ref.56 108 _{τ}*n= 9, τp*= 46 2.4· 10−11 –
Ref.57 5.3· 108_{, 5.7}_{· 10}9 _{12.3}_{− 6.4} _{10}−10 _{–} _{440}
Ref.58 – 44 10−11 10−30 450
Ref.59 2· 1014_{cm}−3 _{100} _{2}_{· 10}−11 _{1.5}_{· 10}−30 _{407}
Ref.30 – – 10−10 8· 10−29 460
Ref.60 – 210 1.2· 10−12 3.5· 10−31 green
Ref.60 – 400 2· 10−12 3.5· 10−31 green
Ref.28 – 50 7· 10−11 10−29 430
Ref.61 – 35− 191 – – 460
Ref.62 – 20− 40 – 5· 10−33 520
Ref.63 5.3· 108_{, 5.7}_{· 10}9 _{10} _{–} _{–}
Ref.64 – 24 3· 10−12 4.5· 10−31 violet
Ref.65 – 0.2− 1 – 1.8− 0.2 · 10−31
Ref.66 – 14− 170 3− 6 · 10−12 0.8− 1 · 10−31 440− 470

### 0

### 5

### 10

### 15

### 20

### 25

### 30

### 35

### 40

### 0

### 0.1

### 0.2

### 0.3

### 0.4

### 0.5

### 0.6

### 0.7

### 0.8

### 0.9

### 1

### Current density, A/cm

2### IQ

### E

*FIG. 15. Normalized simulated IQE (symbols) and measured L/I (lines) as functions of the injection current density in a*
*LDD (solid lines) and HDD (dashed lines) LED at T*= 15◦*C (black lines) and T*= 120◦C (red lines). The non-normalized
value of the maximum simulated IQE is 91%.

*in the LDD and HDD case, the ratio between the present estimates of the C coefficients at 15*◦C
and 120◦C is approximately equal to the ratio between the corresponding absolute temperatures.
If current crowding effects were neglected when comparing experiments and simulations, i.e. if
*fJ,ring≈ fL,ring≈ 1 were assumed, C would be underestimated by a factor ≈1.5÷1.9 (see comment*

at the end of SectionIII A).

*A comparison between measured and simulated IQE(J; T) with the “optimal”* *τSRH* *and C*

values is shown in Fig.15. Fig.16reports the experimental and simulated EL spectra for different
temperatures and currents in a LDD and HDD LED, respectively; for recent comparable experimental
studies on the dependence of *λ*peak on current and temperature, see e.g. Refs.80–82. It is worth

mentioning that, for a realistic description of radiative emission, it has been essential here to take
into account the broadening of interband transitions due to inhomogeneities in QW thickness and
composition.83–85 _{This can be appreciated from Fig.}_{17}_{, which compares simulated EL spectra at}

different temperatures with and without broadening in a LDD LED. The spectra are normalized, as
the adopted model for broadening does not affect the total generated optical power or the IQE. The
inclusion of many-body Coulomb interactions86–92 as implemented in the present versions of the
*simulators has not resulted, with the exception of Eg*renormalization, in a real improvement in their

predictive capabilities, due to the large set of widely-adjustable empirical parameters involved in the corresponding models.

**V. UNCERTAINTY ASSESSMENT**

While a systematic uncertainty quantification is beyond the reach of the present analysis of GaN-based LEDs, we will attempt here a critical discussion of the results derived in SectionIV. Our focus will be on what we consider the weakest points of the DD modeling framework, whose combined

400 450 500 550
0
0.1
0.2
0.3
0.4
0.5
0.6
0.7
0.8
0.9
1
Wavelength, nm
E
L
in
te
ns
it
y,
a
.u.
LDD, 15*◦*C, exp.
LDD, 120*◦*C, exp
LDD, 15*◦*C
LDD, 120*◦*C
4000 450 500 550
0.1
0.2
0.3
0.4
0.5
0.6
0.7
0.8
0.9
1
Wavelength, nm
E
L
in
te
ns
it
y,
a
.u.
LDD, 15*◦*C, exp.
LDD, 120*◦*C, exp
LDD, 15*◦*C
LDD, 120*◦*_{C}
4000 450 500 550
0.1
0.2
0.3
0.4
0.5
0.6
0.7
0.8
0.9
1
Wavelength, nm
E
L
in
te
ns
it
y,
a
.u.
HDD, 15*◦*C, exp.
HDD, 120*◦*C, exp.
HDD, 15*◦*_{C}
HDD, 120*◦*_{C}
4000 450 500 550
0.1
0.2
0.3
0.4
0.5
0.6
0.7
0.8
0.9
1
Wavelength, nm
E
L
in
te
ns
it
y,
a
.u.
HDD, 15*◦*C, exp.
HDD, 120*◦*C, exp.
HDD, 15*◦*_{C}
HDD, 120*◦*_{C}

*FIG. 16. Experimental (solid lines) and simulated (dashed lines) EL spectra in a LDD (top) and HDD (bottom) LED at T*=
15◦*C (black lines) and T*= 120◦*C (red lines) for a current density (left) J*= 8 A/cm2_{and (right) J}_{= 40 A/cm}2_{(corresponding}

*to I= 20 mA and I = 100 mA, respectively).*

limitations could determine, in particular, a severe overestimation of the Auger-like coefficient also beyond the present case study.

**A. Carrier transport across the active region**

In the previous analysis, a standard DD model for carrier transport across the active region has
been adopted, not including carrier flyover (ballistic transport)13–15,24 _{or Auger-induced leakage.}17

The dependence of carrier velocity on the electric field has been approximated with a Canali-like
description93 _{using state-of-the-art model parameters.}94–96 _{We have also experimented modified}

transferred-electron models97_{as well as hydrodynamic and energy-balance descriptions,}98 _{without}

noticeable improvements in the predictive capabilities of the simulator.

Among “quantum–corrected” transport models, a well-established approach available in most
commercial simulators involves the use of separate continuity equations for carriers in unconfined
bulk states (3D) and in bound QW states (2D).99This split-state description, separating the 3D and
2D quasi-Fermi levels in the active region, requires the definition of an appropriate
recombination-like coupling term, in turn involving a set of time constants*τ*QWassociated with the capture/escape

processes.100,101_{A recent body of work using split-state models in InGaN-based LEDs}16,24,102,103

suggests that capture time constants *τ*QW≈ 10−6 s are required in order to obtain realistic IQE

values if other loss mechanisms (Auger recombination in particular) are assumed to be negligible.
The need of such long*τ*QW has led the authors of Ref.24 to rule out incomplete QW capture

(at least, in its present formulation) as a possible droop mechanism. A similar conclusion seems appropriate also in the case of the present LED structures, since not only low capture rates have to

### 400

### 0

### 450

### 500

### 550

### 0.1

### 0.2

### 0.3

### 0.4

### 0.5

### 0.6

### 0.7

### 0.8

### 0.9

### 1

### Wavelength, nm

### E

### L

### in

### te

### ns

### it

### y,

### a

### .u.

*FIG. 17. Simulated EL spectra in a LDD LED at T*= 15◦*C (black lines) and T*= 120◦*C (red lines) for a current density J*=
40 A/cm2_{(corresponding to I}_{= 100 mA) with (solid lines) and without (dashed lines) including inhomogeneous broadening.}

0 5 10 15 20 25 30 35 40 0 0.1 0.2 0.3 0.4 0.5 0.6 0.7 0.8 0.9 1

Current density, A/cm2

IQ
E
experimental
no QT*C = 2.7 · 10−30*cm6_{s}*−1*
no QT*C = 2.7 · 10−31*_{cm}6_{s}*−1*
QT*C = 2.7 · 10−31*_{cm}6_{s}*−1 _{τ}*

*QW*=5

*·10−7*

_{s}QT

*C = 2.7 · 10−31*

_{cm}6

_{s}

*−1*

_{τ}*QW*=1

*·10−7*

_{s}QT

*C = 2.7 · 10−31*cm6

_{s}

*−1*=5

_{τ}_{QW}*·10−8*s 0 5 10 15 20 25 30 35 40 0 0.1 0.2 0.3 0.4 0.5 0.6 0.7 0.8 0.9 1

Current density, A/cm2

IQ
E
experimental
no QT*C = 5.7 · 10−30*cm6_{s}*−1*
no QT*C = 5.7 · 10−31*_{cm}6_{s}*−1*
QT*C = 5.7 · 10−31*_{cm}6_{s}*−1 _{τ}*

*QW*= 5

*· 10−7*

_{s}QT

*C = 5.7 · 10−31*

_{cm}6

_{s}

*−1*

_{τ}*QW*= 1

*· 10−7*

_{s}QT

*C = 5.7 · 10−31*cm6

_{s}

*−1*= 5

_{τ}_{QW}*· 10−8*s

*FIG. 18. Simulated (non-normalized) IQE at T*= 15◦*C (left) and T*= 120◦C (right) as a function of the injection current
density in a LDD LED for different values of the capture time*τ*QW*and a C coefficient set to a value equal to 1/10 of the*

corresponding “best fit” value listed in TableI*. Also reported, as a reference, are the experimental L/I (black solid lines) and*
the corresponding “optimal” simulated IQE with no split-state model (red solid lines) rescaled from Fig.15.

be assumed (*τ*QW≈ 10−7s), but also the IQE dependence on current density and temperature cannot

be satisfactorily reproduced when long*τ*QWare used in the simulations (see Fig.18).

**B. Spontaneous emission**

In the previous Sections, spontaneous emission has been calculated with the present APSYS
* default parameters of the valence band k· p Hamiltonian, reported in Table* IIand derived from

TABLE II. Material parameters of GaN and InN used in the present simulations.

Parameter GaN InN

*a, Å* 3.1892 3.5446
*c, Å* 5.185 5.718
*Egat T*= 0 K, eV 3.507 0.735
*α, meV K*−1 _{0.909} _{0.245}
*β, K* 830 624
*χ, eV* 4.07 5.9272
*so*, meV 14 1
*cr*, meV 19 41
*ε*0 9.5 15
*m**e* 0.20 0.065
*m*⊥*e* 0.20 0.065
*A*1 −6.56 −8.21
*A*2 −0.91 −0.68
*A*3 5.65 7.57
*A*4 −2.83 −5.23
*A*5 −3.13 −5.11
*A*6 −4.86 −5.96
*D*1, eV −3.0 −3.0
*D*2, eV 3.6 3.6
*D*3, eV 8.82 8.82
*D*4, eV −4.41 −4.41
*D*5, eV −4.0 −2.33
*D*6, eV −5.0770 −0.3536
*c*11, GPa 390 271
*c*12, GPa 145 124
*c*13, GPa 106 92
*c*33, GPa 398 224
*c*44, GPa 105 46
*PSP*, C m−2 −0.034 −0.042
*μn*, cm2V−1s−1 300
*μp*, cm2V−1s−1 10

Ref.105for GaN and Ref.106for InN. However widely adopted, those parameter values are affected
by a considerable uncertainty, which directly affects the LED characteristics. As a demonstration
of the importance for device simulation of the description of the valence bands near*, Fig.*19

compares the computed IQE and EL spectra corresponding to the default band parameters and to a
* more recent k· p model derived from many-body perturbation theory in the G*0

*W*0approximation.104

* The newer k· p model, in particular its larger crystal-field splitting of GaN, leads to a nonnegligible*
decrease in both the EL intensity and the IQE at all injection currents; if used in SectionIV, it would

*have led to significantly lower “optimal” estimates of both the A and C coefficients.*

**C. Auger recombination and Auger-related processes**

Fig.20, reporting the simulated IQE as a function of the injection current for different values
*of the C Auger-like coefficient and of the TDD-SRH-like lifetime, could be used to assert our*
confidence in the nonradiative recombination coefficients estimated from the analysis presented in
SectionIV.

*The order of magnitude of our A and C values is indeed in general agreement with several*
simulation studies discussing Auger effects on LED droop3,4,23,24,47,107 _{and recent experimental}

studies on Auger recombination, focusing on its temperature108_{and composition}65,66 _{dependence}

and reaffirming the importance of Auger processes in the blue spectral range. Notably, the Auger-like coefficient determined in the present LED study is increasing with temperature, i.e. it would

### 0

### 5

### 10

### 15

### 20

### 25

### 30

### 35

### 40

### 0

### 0.1

### 0.2

### 0.3

### 0.4

### 0.5

### 0.6

### 0.7

### 0.8

### 0.9

### Current density, A/cm

2### IQ

### E

### 400

### 0

### 450

### 500

### 550

### 0.2

### 0.4

### 0.6

### 0.8

### 1

### Wavelength, nm

*FIG. 19. Simulated (non-normalized) IQE at T*= 15◦C as a function of the injection current density in a LDD LED for the
default band parameters reported in TableII(solid line) and the alternative values proposed in Ref.104(dashed line). The
*corresponding EL spectra at J*= 40 A/cm2_{(I}_{= 100 mA) are reported in the inset.}

0 5 10 15 20 25 30 35 40 0 0.1 0.2 0.3 0.4 0.5 0.6 0.7 0.8 0.9 1

Current density, A/cm2

IQ
E
LDD experimental
HDD experimental
LDD*C = 2.7 · 10−29*cm6_{s}*−1*
LDD*C = 2.7 · 10−30*cm6_{s}*−1*
LDD*C = 2.7 · 10−31*cm6_{s}*−1*
HDD*C = 5.7 · 10−29*cm6_{s}*−1*
HDD*C = 5.7 · 10−30*_{cm}6_{s}*−1*
HDD*C = 5.7 · 10−31*_{cm}6_{s}*−1*
0 5 10 15 20 25 30 35 40
0
0.1
0.2
0.3
0.4
0.5
0.6
0.7
0.8
0.9
1

Current density, A/cm2

IQ
E
LDD experimental
HDD experimental
LDD*τn*=*τp*= 9*· 10−6*_{s}
LDD*τn*=*τp*= 9*· 10−7*_{s}
LDD*τn*=*τp*= 9*· 10−8*s
HDD*τn*=*τp*= 1*.5 · 10−7*_{s}
HDD*τn*=*τp*= 1*.5 · 10−8*_{s}
HDD*τn*=*τp*= 1*.5 · 10−9*s

*FIG. 20. Simulated (non-normalized) IQE at T*= 15◦C as a function of the injection current density for different values of
*the C Auger-like coefficient (left) and of the TDD-related SRH lifetimes (right). Experimental (normalized) L/I values are*
reported as references.

be compatible with Auger processes in InGaN/GaN QWs rather than with density-activated defect recombination or leakage from the active region, both decreasing with increasing temperature.26,29,45

However, in our opinion, an accurate determination of the actual Auger rates remains elusive to
a combined experimental and simulation analysis based on state-of-the-art DD-based optoelectronic
*CAD tools, not only because the applicability of the ABC model to QWs is somehow questionable,*27

but also on account of possible enhancements of Auger recombination by Coulomb interactions109

### 0

### 5

### 10

### 15

### 20

### 25

### 30

### 35

### 40

### 0

### 0.1

### 0.2

### 0.3

### 0.4

### 0.5

### 0.6

### 0.7

### 0.8

### 0.9

### 1

### Current density, A/cm

2### IQ

### E

*FIG. 21. Simulated (non-normalized) IQE at T*= 15◦C as a function of the injection current density for different thickness
and In molar fraction of the QWs: 5 nm, 15% (solid); 2 nm, 15% (dashed), 2 nm, 20% (dashed-dotted). Experimental
*(normalized) L/I values are reported as references.*

also strongly affected by the microscopic details of the MQW heterostructures. If the relationship
between recombination coefficients in bulk and in QWs is not better explored, beyond the attempt
presented in Ref.110*, the very “portability” of C between different devices is dubious.*22 _{Direct}

* calculations of Auger recombination in QW structures, usually based on k· p models, agree in*
suggesting the importance of QW composition profiles77,111

_{and polarization fields}112

_{on the direct}

process rates. Moreover, fluctuations of the In molar fraction across the active region113,114_{could}

have significant effects on both leakage and Auger recombination.115,116

Even assuming an ideally uniform QW profile across the device, as we have done in the previous
*Sections, the determination of C is significantly influenced by the uncertainties on QW thickness*
and composition. As an example, Fig. 21 compares the IQE corresponding to the nonradiative
recombination coefficients estimated in the previous Section (with the “worst case” 5 nm-thick
In0.15Ga0.85N QWs) and the results obtained assuming thinner (2 nm) and deeper (up to 0.20

In molar fraction) QWs. Electron leakage and current crowding are minimally affected by these
*changes, while the use of the worst-case-geometry A and C coefficients with the thinner QWs leads*
*to a significantly larger droop, and the C estimate could be reduced approximately by a factor 3 with*
2 nm-thick In0.2Ga0.8N QWs.

In addition to these uncertainties, recent modeling work17_{suggests that experimentally-derived}

*C values could overestimate the real ones up to a factor 2 since they do not take into account *
Auger-induced leakage effects. Finally, possible non-Auger contributions to the Auger-like coefficients
could derive from photon quenching mechanisms117_{or from strong nolinearities in the n-dependence}

of SRH-like recombination processes determined by multiple-level defects,76 _{and would further}

hamper the discrimination between Auger and other nonradiative mechanisms from an analysis of the LED characteristics.

**VI. CONCLUSIONS**

After a discussion of some important pitfalls stemming from 1D and 2D simulation of LED
*structures – foremost the possible incorrect determination of the C coefficient in the presence of*
current crowding – we have presented a combined experimental and simulative study on InGaN/GaN
LEDs where a seeming excellent match between measured and calculated IQE characteristics and
EL spectra has been achieved over a wide range of temperatures and operating currents, by using
*as the only fitting parameters the A and C coefficients conventionally associated with SRH-like and*
Auger recombination.

However, even if the present study is based on a large and consistent set of experimental
*data, we have shown that the estimates of A and especially C are affected by large error margins*
because of the many sources of uncertainty, related not only to device structure and technological
details (distribution, activation and ionization of dopant species; composition profiles of QWs and
barriers in the active region; uniformity of contacts; parasitic resistances and other interface effects;
etc.) and to material parameters (band offsets and polarization charges at heterojunctions, energy
gap and electronic structure of GaN and InGaN in presence of strain, defects, nonideal interfaces,
etc.), but also to a possibly inadequate description of microscopic processes in the active region
(radiative recombination, intra- and inter-subband carrier scattering, capture/escape between bound
and unbound states, carrier flyover and tunneling etc.) and of their problematic inclusion in a
device-level DD CAD suite.

*These uncertainties are compounded by the nontrivial relationship between the bulk C coefficient*
used in the simulations and the corresponding 2D Auger rate, and by the possible role played by
non-Auger recombination mechanisms with a strong nonlinear dependence on the carrier density;
* a calculation approach for QW structures “beyond k· p” is needed*68,118,119

_{also in order to take}

advantage of possible polarization-engineering opportunities.112,120,121

The prime requisite for a better understanding of experimental information is probably an
improved description of carrier transport across the active region. Promising efforts are represented
by momentum-resolved models23,122and analytic-band Monte Carlo (MC) transport simulations,123
but the need for a full-band MC approach (FBMC, possibly integrated with microscopic models of
radiative and nonradiative recombination processes) is apparent, especially after the recent debate
following the proposed identification of Auger recombination as the dominant mechanism in droop
from electron emission spectroscopy experiments,124_{where FBMC analysis has suggested that the}

LED structure under investigation was probably unsuitable to recover an Auger signature.125

**ACKNOWLEDGMENTS**

The authors thank Simone Chiaria, Andrew Phillips and Michel Lestrade for useful discussions, Simone Vaccari and Marco Ferretti for their contribution to the experimental characterization. The work at Politecnico di Torino and Boston University was supported in part by the U.S. Army Research Laboratory through the Collaborative Research Alliance (CRA) for MultiScale multidisciplinary Modeling of Electronic materials (MSME).

**APPENDIX**

**1. Model parameters**

The nominal values of the material parameters used in the present simulations are listed in Table

II(see also Refs.47,106,126, and127*), where a and c are the lattice constants, Eg* is the energy

gap,*α and β are the coefficients of the Varshni model for the temperature dependence of Eg*,106*χ*

is the electron affinity,*so* and*cr*are the spin-orbit and crystal-field splitting,*ε*0 is the relative

*dielectric constant, m**e* *and m*⊥*e* are the longitudinal and transverse components of the electron

*effective mass, A*1*. . . A*6 * are the Luttinger parameters of the k· p Hamiltonian, D*1

*. . . D*6 are the

*valence band deformation potentials, c*11*. . . c*44*are the elastic constants for wurtzite materials, PSP*is

the spontaneous polarization,*μn, p*are the electron and hole mobilities (assumed to be independent

the values of the binary compounds has been used for all In*x*Ga1−xN parameters, with the exception

*of Eg* *and PSP, where a quadratic correction x(1* *− x)b has been included, with bowing factors b*

equal to 3.0 eV and -0.038 C m−2, respectively. A conduction band offset*Ec*/*Eg*= 0.67 has been

assumed for all heterojunctions, regardless of the In molar fraction.

1_{M. H. Crawford,}_{IEEE J. Select. Topics Quantum Electron.}_{15, 1028 (2009).}

2_{A. Laubsch, M. Sabathil, W. Bergbauer, M. Strassburg, H. Lugauer, M. Peter, S. Lutgen, N. Linder, K. Streubel, J. Hader,}

J. V. Moloney, B. Pasenow, and S. W. Koch,Phys. Stat. Sol. (c)**6, S913 (2009).**
3_{U. ¨}¨ _{Ozg¨ur, H. Liu, X. Li, X. Ni, and H. Morkoc¸,}_{Proc. IEEE}_{98, 1180 (2010).}

4_{J. Piprek,}_{Phys. Stat. Sol. (a)}_{207, 2217 (2010).}

5_{J. Cho, E. F. Schubert, and J. K. Kim,}_{Laser & Photon. Rev.}_{7, 408 (2013).}

6_{G. Verzellesi, D. Saguatti, M. Meneghini, F. Bertazzi, M. Goano, G. Meneghesso, and E. Zanoni,}_{J. Appl. Phys.}_{114,}

071101 (2013).

7_{J. Piprek, and S. Li, in Optoelectronic Devices: Advanced Simulation and Analysis, edited by J. Piprek (Springer, New}

York, 2005) Chap. 10, pp. 293–312.

8_{S. Y. Karpov, in Nitride Semiconductor Devices: Principles and Simulation, edited by J. Piprek (Wiley-VCH Verlag,}

Weinheim, 2007) Chap. 14, pp. 303–325.

9_{N. I. Bochkareva, V. V. Voronenkov, R. I. Gorbunov, A. S. Zubrilov, Y. S. Lelikov, P. E. Latyshev, Y. T. Rebane, A. I.}

Tsyuk, and Y. G. Shreter,Appl. Phys. Lett.**96, 133502 (2010).**

10_{S. Huang, Y. Xian, B. Fan, Z. Zheng, Z. Chen, W. Jia, H. Jiang, and G. Wang,}_{J. Appl. Phys.}** _{110, 064511 (2011).}**
11

_{H. Zhao, G. Liu, R. A. Arif, and N. Tansu, Semiconductor Sci. Tech. 54, 1119 (2010).}12_{T.-S. Kim, B.-J. Ahn, Y. Dong, K.-N. Park, J.-G. Lee, Y. Moon, H.-K. Yuh, S.-C. Choi, J.-H. Lee, S.-K. Hong, and J.-H.}

Song,Appl. Phys. Lett.**100, 071910 (2012).**

13_{X. Ni, X. Li, J. Lee, S. Liu, V. Avrutin, ¨}_{U. ¨}_{Ozg¨ur, H. Morkoc¸, and A. Matulionis,}_{J. Appl. Phys.}** _{108, 033112 (2010).}**
14

_{M. V. Kisin and H. S. El-Ghoroury,}

_{Phys. Stat. Sol. (c)}

_{8, 2264 (2011).}15_{U. ¨}_{¨} _{Ozg¨ur, X. Ni, X. Li, J. Lee, S. Liu, S. Okur, V. Avrutin, A. Matulionis, and H. Morkoc¸,}_{Semiconductor Sci. Tech.}_{26,}

014022 (2011).

16_{C. S. Xia, Z. M. S. Li, Y. Sheng, L. W. Cheng, W. D. Hu, and W. Lu,}_{Opt. Quantum Electron.}** _{45, 597 (2013).}**
17

_{M. Deppner, F. R¨omer, and B. Witzigmann,}

_{Phys. Stat. Sol. RRL}

_{6, 418 (2012).}18_{H. Li, X. Liu, J. Wang, D. Jin, H. Zhang, S. Yang, S. Liu, W. Mao, Y. Hao, Q. Zhu, and Z. Wang,}_{J. Appl. Phys.}_{112,}

113712 (2012).

19_{L. Dong, J. V. Mantese, V. Avrutin, ¨}_{U. ¨}_{Ozg¨ur, H. Morkoc¸, and S. P. Alpay,}_{J. Appl. Phys.}** _{114, 043715 (2013).}**
20

_{S.-I. Park, J.-I. Lee, D.-H. Jang, H.-S. Kim, D.-S. Shin, H.-Y. Ryu, and J.-I. Shim,}

_{IEEE J. Quantum Electron.}

_{48, 500}(2012).

21_{M. A. Caro, S. Schulz, and E. P. O’Reilly,}_{Phys. Rev. B}** _{88, 214103 (2013).}**
22

_{P. Blood,}

_{IEEE J. Quantum Electron.}

_{36, 354 (2000).}23_{W. W. Chow,}_{Opt. Express}_{19, 21818 (2011).}

24_{D. Saguatti, L. Bidinelli, G. Verzellesi, M. Meneghini, G. Meneghesso, E. Zanoni, R. Butendeich, and B. Hahn,}_{IEEE}

Trans. Electron Devices**59, 1402 (2012).**

25_{I.-G. Choi, D.-P. Han, J. Yun, K. S. Kim, D.-S. Shin, and J.-I. Shim,}_{Appl. Phys. Express}** _{6, 052105 (2013).}**
26

_{J. Hader, J. V. Moloney, and S. W. Koch,}

_{Appl. Phys. Lett.}

_{99, 181127 (2011).}27_{J. Hader, J. V. Moloney, and S. W. Koch, in}_{SPIE Photonics West, Physics and Simulation of Optoelectronic Devices XIV,}

Vol. 6115, Proceedings of the SPIE (San Jose, CA, 2006) p. 61151T.

28_{A. David and M. J. Grundmann,}_{Appl. Phys. Lett.}** _{96, 103504 (2010).}**
29

_{J. Hader, J. V. Moloney, and S. W. Koch,}

_{Appl. Phys. Lett.}

_{96, 221106 (2010).}30_{Q. Dai, Q. Shan, J. Wang, S. Chhajed, J. Cho, E. F. Schubert, M. H. Crawford, D. D. Koleske, M.-H. Kim, and Y. Park,}

Appl. Phys. Lett.**97, 133507 (2010).**

31_{G.-B. Lin, D. Meyaard, J. Cho, E. F. Schubert, H. Shim, and C. Sone,}_{Appl. Phys. Lett.}_{100, 161106 (2012).}

32_{G.-B. Lin, Q. Shan, A. J. Birkel, J. Cho, E. F. Schubert, M. H. Crawford, K. R. Westlake, and D. D. Koleske,}_{Appl. Phys.}

Lett.**101, 241104 (2012).**

33_{Y. Lin, Y. Zhang, Z. Liu, L. Su, J. Zhang, T. Wei, and Z. Chen,}_{Appl. Phys. Lett.}_{101, 252103 (2012).}

34_{All simulation results discussed in Section}_{III}_{have been determined with the “optimal” SRH lifetimes and Auger}

coefficients listed in TableI.

35_{X. Guo and E. F. Schubert,}_{J. Appl. Phys.}_{90, 4191 (2001).}

36_{H. Kim, S.-J. Park, and H. Hwang,}_{IEEE Trans. Electron Devices}** _{48, 1065 (2001).}**
37

_{V. K. Malyutenko, S. S. Bolgov, and A. D. Podoltsev,}

_{Appl. Phys. Lett.}

**38**

_{97, 251110 (2010).}_{Y. Y. Kudryk and A. V. Zinovchuk,}

_{Semiconductor Sci. Tech.}

**39**

_{26, 095007 (2011).}_{K.-S. Lee,}

_{Phys. Stat. Sol. (a)}

_{209, 2630 (2012).}40_{V. Malyutenko, S. Bolgov, and A. Tykhonov,}_{IEEE Photon. Technol. Lett.}_{24, 1124 (2012).}

41_{Y. Zhang, H. Zheng, E. Guo, Y. Cheng, J. Ma, L. Wang, Z. Liu, X. Yi, G. Wang, and J. Li,}_{J. Appl. Phys.}_{113, 014502}

(2013).

42_{Y. Y. Kudryk, A. K. Tkachenko, and A. V. Zinovchuk,}_{Semiconductor Sci. Tech.}** _{27, 055013 (2012).}**
43

_{C.-K. Li and Y.-R. Wu,}

_{IEEE Trans. Electron Devices}

_{59, 400 (2012).}44_{E. Jung, S. Kim, and H. Kim,}_{IEEE Electron Device Lett.}** _{34, 277 (2013).}**
45

_{J. Piprek and S. Li,}

_{Opt. Quantum Electron.}

_{42, 89 (2010).}47_{S. Chiaria, E. Furno, M. Goano, and E. Bellotti,}_{IEEE Trans. Electron Devices}_{57, 60 (2010).}

48_{M. Meneghini, S. Vaccari, A. Garbujo, N. Trivellin, D. Zhu, C. J. Humphreys, M. Calciati, M. Goano, F. Bertazzi, G.}

**Ghione, E. Bellotti, G. Meneghesso, and E. Zanoni, Japan. J. Appl. Phys. 52, 08JG09 (2013).**

49_{In the following, the total optical power P}

op*generated inside the active region has been taken into account to determine*

*the internal quantum efficiency (IQE), but for better consistency with the experimental L/I curves one could consider only*
the power emitted from the top surface of the mesa.

50_{J. Piprek, T. M. Katona, S. P. DenBaars, and S. Li, in}_{SPIE Photonics West, Light-Emitting Diodes: Research, }

*Manufac-turing, and Applications VIII, Vol. 5366, Proceedings of the SPIE (San Jose, CA, 2004) pp. 127–136.*

51_{S. Li, Z. Q. Li, O. Shmatov, C. S. Xia, and W. Lu, in}_{2005 MRS Fall Meeting, Vol. 892, Materials Research Society}

Symposium Proceedings (MRS, 2005) pp. 0892–FF12–12.

52_{Y. Sheng, O. Shmatov, and Z. M. S. Li, in}_{6th International Conference on Numerical Simulation of Optoelectronic}

*Devices (NUSOD ’06)*(Singapore, 2006) pp. 19–20.

53_{M. Othman, S. Ahmad, F. Sa’ad, A. Alias, A. Aziz, and M. Hashim, in}_{2012 IEEE International Conference on Control}

*System, Computing and Engineering (ICCSCE)*(Penang, Malaysia, 2012) pp. 530–534.

54_{Y. Sheng, C. S. Xia, Z. M. S. Li, and L. W. Cheng, in}_{12th International Conference on Numerical Simulation of}

*Optoelectronic Devices (NUSOD 2012)*(Shanghai, China, 2012) pp. 23–24.

55_{C.-K. Li, H.-C. Yang, T.-C. Hsu, Y.-J. Shen, A.-S. Liu, and Y.-R. Wu,}_{J. Appl. Phys.}** _{113, 183104 (2013).}**
56

_{K. A. Bulashevich, V. F. Mymrin, S. Y. Karpov, I. Zhmakin, and A. Zhmakin,}

_{J. Comp. Phys.}

**57**

_{213, 214 (2006).}_{M. F. Schubert, S. Chhajed, J. K. Kim, E. F. Schubert, D. D. Koleske, M. H. Crawford, S. R. Lee, A. J. Fischer, G. Thaler,}

and M. A. Banas,Appl. Phys. Lett.**91, 231114 (2007).**

58_{M. Meneghini, N. Trivellin, G. Meneghesso, E. Zanoni, U. Zehnder, and B. Hahn,}_{J. Appl. Phys.}** _{106, 114508 (2009).}**
59

_{M. Zhang, P. Bhattacharya, J. Singh, and J. Hinckley,}

_{Appl. Phys. Lett.}

_{95, 201108 (2009).}60_{A. Laubsch, M. Sabathil, J. Baur, M. Peter, and B. Hahn,}_{IEEE Trans. Electron Devices}_{57, 79 (2010).}

61_{D. S. Meyaard, Q. Shan, Q. Dai, J. Cho, E. F. Schubert, M.-H. Kim, and C. Sone,}_{Appl. Phys. Lett.}** _{99, 041112 (2011).}**
62

_{H. Zhao, G. Liu, J. Zhang, J. D. Poplawsky, V. Dierolf, and N. Tansu,}

_{Opt. Express}

_{19, A991 (2011).}63_{S. Chhajed, J. Cho, E. F. Schubert, J. K. Kim, D. D. Koleske, and M. H. Crawford,}_{Phys. Stat. Sol. (a)}** _{208, 947 (2011).}**
64

_{W. G. Scheibenzuber, U. T. Schwarz, L. Sulmoni, J. Dorsaz, J.-F. Carlin, and N. Grandjean,}

_{J. Appl. Phys.}

_{109, 093106}(2011).

65_{M. Brendel, A. Kruse, H. J¨onen, L. Hoffmann, H. Bremers, U. Rossow, and A. Hangleiter,}_{Appl. Phys. Lett.}_{99, 031106}

(2011).

66_{D. Schiavon, M. Binder, M. Peter, B. Galler, P. Drechsel, and F. Scholz,}_{Phys. Stat. Sol. (b)}** _{250, 283 (2013).}**
67

_{F. Bertazzi, M. Goano, and E. Bellotti,}

_{Appl. Phys. Lett.}

_{101, 011111 (2012).}68_{F. Bertazzi, X. Zhou, M. Goano, G. Ghione, and E. Bellotti,}_{Appl. Phys. Lett.}** _{103, 081106 (2013).}**
69

_{S. Y. Karpov and Y. N. Makarov,}

_{Appl. Phys. Lett.}

_{81, 4721 (2002).}70_{T. Langer, A. Kruse, F. A. Ketzer, A. Schwiegel, L. Hoffmann, H. J¨onen, H. Bremers, U. Rossow, and A. Hangleiter,}

Phys. Stat. Sol. (c)**8, 2170 (2011).**

71_{L. Lu, Y. H. Zhu, Z. T. Chen, and T. Egawa,}_{J. Appl. Phys.}_{109, 113537 (2011).}

72_{A. Armstrong, T. A. Henry, D. D. Koleske, M. H. Crawford, K. R. Westlake, and S. R. Lee,}_{Appl. Phys. Lett.}_{101, 162102}

(2012).

73_{L. C. Le, D. G. Zhao, D. S. Jiang, L. Li, L. L. Wu, P. Chen, Z. S. Liu, Z. C. Li, Y. M. Fan, J. J. Zhu, H. Wang, S. M. Zhang,}

and H. Yang,Appl. Phys. Lett.**101, 252110 (2012).**

74_{S.-K. Lee, H. S. Lim, J.-H. Lee, H.-S. Kwack, H. K. Cho, H.-K. Kwon, and M. S. Oh,}_{J. Appl. Phys.}** _{111, 103115 (2012).}**
75

_{D.-Y. Lee, S.-H. Han, D. J. Lee, J. W. Lee, D.-J. Kim, Y. S. Kim, S.-T. Kim, and J.-Y. Leem,}

_{Appl. Phys. Lett.}

_{102, 011115}(2013).

76_{N. A. Modine, A. M. Armstrong, M. H. Crawford, and W. W. Chow,}_{J. Appl. Phys.}** _{114, 144502 (2013).}**
77

_{R. Vaxenburg, E. Lifshitz, and A. L. Efros,}

_{Appl. Phys. Lett.}

_{102, 031120 (2013).}78_{Y. C. Shen, G. O. Mueller, S. Watanabe, N. F. Gardner, A. Munkholm, and M. R. Krames,}_{Appl. Phys. Lett.}_{91, 141101}

(2007).

79_{A. David and M. J. Grundmann,}_{Appl. Phys. Lett.}_{97, 033501 (2010).}

80_{C. Netzel, S. Hatami, V. Hoffmann, T. Wernicke, A. Knauer, M. Kneissl, and M. Weyers,}_{Phys. Stat. Sol. (c)}_{8, 2151}

(2011).

81_{Y. Dong, J.-H. Song, H.-J. Kim, T.-S. Kim, B.-J. Ahn, J.-H. Song, I.-S. Cho, W.-T. Im, Y. Moon, S.-M. Hwang, S.-K.}

Hong, and S.-W. Lee,J. Appl. Phys.**109, 043103 (2011).**

82_{C. Lu, L. Wang, J. Lu, R. Li, L. Liu, D. Li, N. Liu, L. Li, W. Cao, W. Yang, W. Chen, W. Du, C.-T. Lee, and X. Hu,}_{J.}

Appl. Phys.**113, 013102 (2013).**

83_{J. Hader, J. V. Moloney, S. W. Koch, and W. W. Chow,}_{IEEE J. Select. Topics Quantum Electron.}** _{9, 688 (2003).}**
84

_{M. Gladysiewicz, R. Kudrawiec, M. Syperek, J. Misiewicz, M. Siekacz, G. Cywinski, C. Skierbiszewski, and T. Suski,}

Phys. Stat. Sol. (c)**8, 2273 (2011).**

85_{M. Gladysiewicz, R. Kudrawiec, J. Misiewicz, M. Siekacz, G. Cywinski, and C. Skierbiszewski,}_{Phys. Stat. Sol. (c)}_{8,}

2282 (2011).

86_{H. Haug and S. W. Koch,}_{Phys. Rev. A}_{39, 1887 (1989).}

87_{W. W. Chow, A. Knorr, and S. W. Koch,}_{Appl. Phys. Lett.}_{67, 754 (1995).}

88_{A. Girndt, F. Jahnke, S. W. Koch, and W. W. Chow,}_{Mater. Sci. Eng. B}_{50, 174 (1997).}

89_{W. W. Chow and S. W. Koch, Semiconductor-Laser Fundamentals. Physics of the Gain Materials (Springer-Verlag, Berlin,}

1999).

90_{S.-H. Park, D. Ahn, and J.-W. Kim,}_{Appl. Phys. Lett.}_{94, 041109 (2009).}